Text of Measuring True Young’s Modulus of a Cantilevered Nanowire
Measuring True Young’s Modulus of a Cantilevered Nanowire: Effect of Clamping on Resonance Frequency
Qingquan Qin , Feng Xu , Yongqing Cao , Paul I. Ro , and Yong Zhu *
The effect of clamping on resonance frequency and thus measured Young’s modulus of nanowires (NWs) is systematically investigated via a combined experimental and simulation approach. ZnO NWs are used in this work as an example. The resonance tests are performed in situ inside a scanning electron microscope and the NWs are cantilevered on a tungsten probe by electron-beam-induced deposition (EBID) of hydrocarbon. EBID is repeated several times to deposit more hydrocarbons at the same location. The resonance frequency increases with the increasing clamp size until approaching that under the “fi xed” boundary condition. The critical clamp size is identifi ed as a function of NW diameter and NW Young’s modulus. This work: 1) exemplifi es the importance of considering the effect of clamping in measurements of Young’s modulus using the resonance method, and 2) demonstrates that the true Young’s modulus can be measured if the critical clamp size is reached. Design guidelines on the critical clamp size are provided. Such design guidelines can be extended to other one-dimensional nanostructures such as carbon nanotubes.
One-dimensional (1D) nanostructures such as nanowires
(NWs) and nanotubes are critical building blocks of nanotech-
nologies. [ 1 ] They exhibit outstanding mechanical properties in
addition to electrical, thermal and optical properties. As such,
they have been demonstrated in a broad range of applications
including nanosensors, nanoelectromechanical systems, [ 2 ] and
nanoscale energy harvesting/storage. [ 3 ] It has been reported
that size-dependent mechanical properties arise as the char-
acteristic dimension approaches sub-100 nm. [ 4 ] Therefore, it is
important to accurately measure their mechanical properties,
which is key to gaining fundamental understanding of surface
effects on such properties.
Mechanical testing of 1D nanostructures is challenging
in spite of recent advances. [ 5 ] Notable experimental methods
include vibration/resonance, [ 4b , 6 ] bending, [ 7 ] tension, [ 8 ] and
Q. Qin , [ + ] F. Xu , [ + ] Dr. Y. Cao , Prof. P. I. Ro , Prof. Y. Zhu Department of Mechanical and Aerospace Engineering North Carolina State University Raleigh, North Carolina 27695-7910, USA E-mail: [email protected]
[ + ] These authors contributed equally to this work
small 2012, DOI: 10.1002/smll.201200314
nanoindentation. [ 9 ] In the resonance test, amplitude and res-
onance frequency of NWs can be measured by microscopy
imaging. Following a simple beam theory, Young’s modulus
of NWs can be calculated. The uncertainty in boundary
condition could lead to considerable errors in the Young’s
modulus. In the bending method, atomic force microscopy
(AFM) is used to defl ect a single NW and measure the load
and displacement simultaneously. However, the AFM tip
might slip from the NW in the cantilevered (single-clamped)
case while the induced axial force might cause a nonlinear
effect that is typically not considered in data reduction in
the double-clamped case. The uniaxial tensile test is the most
straightforward method for mechanical characterization of
bulk materials. Microelectromechanical systems (MEMS)
have recently emerged as a promising tool for in situ electron
microscopy tensile testing of NWs. [ 8b , 10 ] However, the tensile
testing of NWs generally requires specifi c nanomanipulation
and testing procedures, which could be laborious.
Resonance is a simple and widely used method to
measure Young’s modulus of NWs. According to a simple
beam theory, the n th mode resonance frequency of a single-
Figure 1 . a) Schematic of the experimental setup. b) SEM image of a stationary ZnO NW with one end clamped on the tip of the tungsten probe. c) SEM image of the ZnO NW under resonance at the fundamental harmonic mode.
where E is the Young’s modulus, I is the moment of inertia, L
is the beam length, A is the cross-sectional area and ρ is the
beam density. The β n term is the eigenvalue from the charac-
teristic equation: cos β n sin β n + 1 = 0; β 0 = 1.875, β 1 = 4.694, and
β 2 = 7.855 correspond to the fi rst three resonance modes for
any cantilevered beam. [ 11 ] When the resonance frequency is
measured, the Young’s modulus can be calculated according
to Equation (1) . However, Equation (1) assumes the “fi xed”
boundary condition that requires zero displacement and
slope at the “fi xed” end. For NW testing, two methods are
often used to attach NWs to a substrate. The fi rst method is
to grow NWs on top of a substrate. [ 4b ] In this case, it is rea-
sonable to assume a “fi xed” boundary condition. But this
method is limited to those NWs that can be directly grown on
the substrate; plus, such type of NW growth is not trivial. The
second method involves picking up a single NW (e.g., using a
nanomanipulator), attaching it to a substrate and clamping it.
One way for clamping a NW is electron-beam-induced depo-
sition (EBID) of residual hydrocarbon in a scanning electron
microscope (SEM) chamber or intentionally introduced pre-
cursor gas. This method is general and can be applied to any
NWs. However, the clamping materials are compliant, which
leads to a concern whether the boundary condition can be
assumed “fi xed”.
In this paper, we systematically investigate the effect of
clamping on the resonance frequency and thus the Young’s
modulus of ZnO NWs. The reason to study ZnO NWs is
that they are one of the most important functional NWs [ 12 ]
and their mechanical properties have been relatively well
understood. [ 4a , b , e ] In situ mechanical resonance tests of ZnO
NWs were performed inside a SEM, where the NWs were
clamped on a tungsten probe by EBID of hydrocarbon
(available in the SEM chamber). EBID was repeated sev-
eral times to deposit more clamping material on the same
location; after each deposition the resonance frequency was
measured. The resonance frequency increased with the clamp
size initially but then gradually approached a constant value.
Finite element analysis was carried out to simulate the effect
of the clamp size on the NW resonance frequency, which
agreed well with the experimental results. Both experiments
and simulations showed that with suffi cient clamp material,
the resonance frequency converges to that under the “fi xed’
boundary condition (i.e., the “fi xed” boundary condition is
2. Results and Discussion
Figure 1 a shows a schematic of the experimental setup. A
piezoelectric sheet was used to provide mechanical vibration.
The piezoelectric sheet was glued to the SEM sample holder
on one side and a tungsten probe was glued to the other side.
NWs were later clamped on the tungsten probe for vibration
tests. The ZnO NWs used in this work were uniform in dia-
meter along the growth direction. Figure 1 b shows a sta-
tionary ZnO NW with one end clamped on the tip of the
fi rst tungsten probe as mentioned above. Figure 1 c shows the
vibrated NW under resonance. The NWs were only vibrated
The procedure to test the effect of clamping on the res-
onance frequency of ZnO NWs was as follows. First, SEM
images around the resonance frequency of the initially
clamped NW were taken (the resonance frequency was deter-
mined later). EBID was then used again to deposit more car-
bonaceous material at the same clamp location. SEM images
around the new resonance frequency were taken again. The
process of depositing more material at the same clamp loca-
tion and taking SEM images around the new resonance fre-
quency was repeated several times.
Figure 2 a shows the amplitude–frequency characteristics
of a NW after each deposition. Overall, fi ve deposition times
were used for this NW. The deposition line widths were 19,
25, 39, 65, and 79 nm, respectively. It can be seen that the res-
onance frequency increased after each additional deposition,
but approached a constant value after the line width of 65 nm
erlag GmbH & Co. KGaA, Weinheim small 2012, DOI: 10.1002/smll.201200314
Measuring True Young’s Modulus of a Cantilevered Nanowire
Figure 2 . a) The amplitude–frequency characteristics of a NW after each deposition. The curves show the Lorentzian fi ts. b) The resonance frequency of the NW as a function of the clamp width. The inset shows SEM image of the NW clamped by a line pattern (deposited by EBID).
710 720 730 740 750 760 770 780 790
After 1st deposition After 2nd depositionAfter 3rd deposition After 4th depositionAfter 5th deposition
10 20 30 40 50 60 70 80710
Clamp width (nm)
Figure 3 . 3D view of the confi guration used in the simulation including the deposition line and the ZnO NW. The inset shows a magnifi ed view of the middle part of the deposition line.
Table 1 . The dimensions of the NWs and the extrapolated Young’s moduli of the NWs corresponding to their diameters.
NW1 NW2 NW3
Diameter [nm] 55 60 62
Length [ μ m] 7.14 7.04 6.73
Young’s modulus [GPa] 173 168 167
(Figure 2 b). SEM image in the inset of Figure 2 b shows a rep-
resentative line pattern of hydrocarbon (deposited by EBID).
The length of the deposition (clamp) line was measured to
be ∼ 440 nm, which was kept the same in spite of changing
the width. The line width increased after each deposition.
The line width was measured from SEM images, but not the
line thickness. To systematically characterize the dimensions
of the deposition lines, hydrocarbon was deposited on a pol-
ished tungsten foil (similar to the tungsten probe). On the
tungsten foil, SEM and AFM (Park Systems, XE-70) charac-
terization can be conducted to measure the width and thick-
ness of the same deposition line, respectively (see Supporting
Information (SI)). The line thickness was found to increase
with the line width; their relationship is shown in Figure S1d
of the SI.
Finite element analysis (ABAQUS) was used to simu-
late the effect of deposition (clamp) on the resonance
frequency. Figure 3 shows the confi guration used in the
simulation including the deposition line and the ZnO NW.
Fixed boundary condition was applied to the bottom of the
deposition line, and the NW was tied to the deposition line.
20-node quadratic brick elements (C3D20R) and 4-node
linear tetrahedron elements (C3D4) were used for the NW
and the deposition line, respectively. A numerical method,
so-called linear perturbation step, available in ABAQUS was
used to extract the resonance frequencies. The dimensions of
the deposition line used here were obtained from Figure S1d
of the SI; the range of the line width was set to be from
10 to 83 nm while the corresponding thickness ranged from
28 to 117 nm. The cross section of the deposition line was a
parabolic shape (Figure 3 c), which was found to best fi t the
experimental results when compared to other shapes such
as semicircle/rectangle and rectangle (see SI). The length of
the deposition line was set to be 440 nm, the same as that
in the experiments. The Young’s modulus of the deposited
material was 40 GPa. [ 13 ] The dimension of each NW was
measured from experiments. The Young’s modulus of ZnO
NWs has been found to depend on the NW diameter and
loading mode (i.e., tension versus bending). [ 4e , 14 ] The Young’s
moduli of NWs used in the simulation were taken from those
under the same loading mode (i.e., resonance tests with NWs
directly grown on a substrate). [ 4b ]
Three NWs were tested in our experiments and each
NW underwent multiple depositions. The dimensions of
these NWs are listed in Table 1 . The length of each NW
was measured from the middle of the deposition line to the
vibrating end of the NW. The Young’s moduli of the NWs
corresponding to their diameters are also listed in the Table 1
(extrapolated from reference [ 4b ] ). Using these values in the
3www.small-journal.comH & Co. KGaA, Weinheim
Q. Qin et al.full papers
Figure 4 . a) Plots of the resonance frequencies of the three NWs versus clamp widths from the experiments, simulation and analytical calculation. In the analytical solution, since the effective NW length decreases with increasing clamp width, the resonance frequency increase slightly. b) Young’s moduli of the three NWs as a function the clamp width, as calculated from the experimental resonance frequencies using the beam theory. The dash lines indicate the Young’s moduli of the NWs under “fi xed” boundary condition.
and simulation results. ZnO NWs have hexagonal cross sec-
tions, so the resonance frequency at the fundamental har-
monic mode can be written as
f0 = β20
where D is the beam diameter (distance between two dia-
metrically opposite vertices for a hexagon). The analytical
results are also plotted in Figure 4 a as dashed lines. Note
that the slight change in the resonance frequency is a result
of the change in effective NW length (due to the increase in
clamp width). The effective NW length (defi ned as the length
from the closer edge of the deposition line to the free end
of the NW) is used in the analytical calculation. Apparently,
with the increase of clamp size, the discrepancy between the
analytical calculation and experiment/simulation decreases.
Especially when the clamp width approaches 80 nm, the
resonance frequencies from experiments and simulations are
almost identical to that from the analytical calculation. Thus,
it is reasonable to conclude that the “fi xed” boundary condi-
tion is met when the clamp width reaches 80 nm or larger, for
the ZnO NWs tested in this work (diameters between 55 and
Figure 4 b plots the measured Young’s moduli of the three
NWs as a function the clamp width, as calculated from the
measured resonance frequencies using Equation (2) . Note
that the effective NW lengths are used in the calculation.
For all the NWs, the Young’s moduli increase with the clamp
size and approach the reported values. [ 4b ] This indicates that
the errors in the Young’s modulus measurement from the
resonance test can be minimized by increasing the deposi-
tion width. Two additional remarks are noted. First, when the
clamp size is small, the resultant error in Young’s modulus
can be as large as 13.4% (for instance, for NW1). The above
analysis provides a rationale behind the low modulus values
reported for ZnO nanobelts and NWs (also using the reso-
nance test). [ 15 ] Among other reasons, the low values might be
caused by the imperfect boundary conditions, in which the
nanostructures were barely attached to a gold ball or tungsten
probe without deposition clamping. Second, the change in
effective NW length causes a slight variation in the calculated
resonance frequency (as shown in dashed lines in Figure 4 a)
and thus Young’s modulus. However, the change in effective
NW length is very small (40 nm versus a typical NW length
of over 6 μ m). According to Equation (2) , the relative error
is less than 2.6% for a measured resonance frequency, which
might be negligible for most applications.
To provide a design guideline for those who might use the
EBID of hydrocarbon for clamping NWs, a parametric study
was further pursued to illustrate the effects of clamp length,
NW diameter and NW Young’s modulus. The clamp length
does not play an important role as long as it exceeds about
4 times of the NW diameter, as shown in Figure S3 of the SI.
But the NW diameter and NW Young’s modulus play impor-
tant roles, thus imposing stringent requirement on the clamp
width to achieve the “fi xed” boundary condition. Figure 5
shows the effect of the NW diameter on the resonance fre-
quency (with a constant NW Young’s modulus of 168 GPa).
erlag GmbH & Co. KGaA, Weinheim small 2012, DOI: 10.1002/smll.201200314
Measuring True Young’s Modulus of a Cantilevered Nanowire
Figure 7 . The critical clamp width as functions of diameter and Young’s modulus of NW. The fi tting plane shows w cr = α D ( E / E hc )
n , with α = 0.786 and n = 0.2.
Figure 5 . Resonance frequency as a function of clamp width for NWs with different diameters (from 15 nm to 120 nm). A constant NW Young’s modulus (168 GPa) is used here. The dash lines indicate the resonance frequencies under “fi xed” boundary condition.
0 20 40 60 80 100 120
Clamp width (nm)
15 nm 30 nm 60 nm
80 nm 100 nm
More details can be seen in Figure S4 of the SI. For each NW
diameter, the NW resonance frequency increases with the
clamp width. The critical clamp width, above which the “fi xed”
boundary condition is reached, appears to be approximately
equal to the NW diameter. Figure 6 shows the effect of the
NW Young’s modulus on the resonance frequency (with a
constant NW diameter of 60 nm). For each Young’s modulus,
the resonance frequency increases with the clamp width. The
critical clamp width appears to increase linearly with the res-
onance frequency under the “fi xed” boundary condition (i.e.,
square root of the NW Young’s modulus according to Equa-
tion (1) ). Note that the critical width is defi ned as the width
when the difference between the calculated (dashed line) and
simulated (dots) resonance frequency of a NW is less than
Figure 6 . Resonance frequency as a function of clamp width for NWs with different Young’s modulus (from 20 GPa to 600 GPa). A constant NW diameter (60 nm) is used here. The dash lines indicate the resonance frequencies under “fi xed” boundary condition.
1% in Figure 5 . It is of additional note that the aspect ratio of
NW (NW length over diameter) does not play an important
role in determining critical clamp width as long as the ratio is
larger than 40, as shown in Figure S5 of the SI.
It becomes clear that the critical clamp width depends
on the NW diameter and the NW Young’s modulus. Figure 7
plots the critical clamp width as a function of the NW dia-
meter and the NW Young’s modulus. A plane fi tting was
applied to the data, and a simple scaling law was extracted
from Figure 7 , viz.,
wcr = αD
where w cr is the critical clamp width, D is the NW diameter, E
is the NW Young’s modulus, E hc is the hydrocarbon Young’s
modulus ( = 40 GPa [ 13 ] ), α is a constant ( = 0.786 in this work)
and n equal to 0.2. The coeffi cient of determination ( R 2 ) using
this fi tting function is 0.97, indicating that the function fi ts the
data very well.
We have systematically investigated the effect of clamping
on the resonance frequency and hence the measured
Young’s modulus of cantilevered NWs by a combined exper-
iment and simulation approach. The resonance tests were
performed in situ inside a SEM with ZnO NWs clamped
on tungsten probes by EBID of hydrocarbon. EBID was
repeated several times to deposit more hydrocarbons at the
same location and the resonance frequencies were measured
after each deposition until a stable resonance frequency was
5www.small-journal.comH & Co. KGaA, Weinheim
Q. Qin et al.full papers
obtained. Finite element analysis was carried out to simu-
late the clamping effect, which agreed well with the experi-
mental results. Initially the resonance frequency increased
rapidly with the clamp size. When the clamp width reached
a critical value, the resonance frequency approached that
under the “fi xed’ boundary condition. Further numerical
simulations were performed to investigate the effect of NW
diameter and Young’s modulus on the clamp size (including
width and length), which led to a simple scaling law that
can be used as guidelines for future designs. Our work
demonstrates that true Young’s modulus can be measured
if the critical clamp size is reached. Also in calculating the
Young’s modulus, it is acceptable to use the nominal NW
length (from the center of the clamp to the vibrating end
of the NW) instead of the effective NW length (from the
closer edge of the deposition line to the vibrating end of the
NW). Our work provides design guidelines on the critical
clamp size, which is useful in accurate measurement of the
Young’s modulus of 1D nanostructures using the resonance
4. Experimental Section
The ZnO NWs were synthesized by the vapor–liquid–solid method on Si/SiO 2 substrates with Au colloids as the catalysts. [ 16 ] The mechanical resonance tests were performed inside an SEM (JEOL 6400F). A nanomanipulator (Klocke Nanotechnik, Germany) with 1 nm resolution and 1 cm travel range in three orthogonal direc-tions was used to pick up protruding NWs from the Si substrate following the procedure outlined by Zhu and Espinosa. [ 8b ] After a ZnO NW was clamped to the second tungsten probe on the nanomanipulator using EBID of carbonaceous materials in the SEM chamber, the NW was pulled away from the Si substrate, moved toward the fi rst tungsten probe (glued to the piezoelec-tric sheet). Using EBID again, the NW was clamped on the tip of the fi rst probe, and then the other clamp was broken off. This depends on the strength difference of the two clamps; the clamp on the second probe is intentionally weaker than that on the fi rst probe. The strength difference was achieved by controlling the deposition time. Note that the second probe broke off from the short end of the NW (Figure 1 a). Subsequently, the piezoelec-tric sheet was excited into mechanical vibration by applying an AC voltage of 0.5 V, which drove mechanical resonance in the attached NW (through the fi rst probe). For mechanically induced resonance of NWs, the frequency of the applied AC signal is the NW’s resonance frequency. The case of electrically induced reso-nance could be more complicated. [ 11 ] Around the resonance fre-quency of each NW, SEM images of the vibrating NW were taken at a number of frequencies, from which the vibration amplitude was measured as a function of the frequency (Figure 2 a). Then the resonance frequency can be determined from the amplitude-frequency plot.
[ 1 ] a) R. H. Baughman , A. A. Zakhidov , W. A. de Heer , Science 2002 , 297 , 787 ; b) W. Lu , C. M. Lieber , J. Phys. D: Appl. Phys. 2006 , 39 , R387 .
[ 2 ] X. L. Feng , R. R. He , P. D. Yang , M. L. Roukes , Nano Lett. 2007 , 7 , 1953 . [ 3 ] a) Z. L. Wang , J. H. Song , Science 2006 , 312 , 242 ; b) C. K. Chan ,
H. L. Peng , G. Liu , K. McIlwrath , X. F. Zhang , R. A. Huggins , Y. Cui , Nat. Nanotechnol. 2008 , 3 , 31 .
[ 4 ] a) F. Xu , Q. Q. Qin , A. Mishra , Y. Gu , Y. Zhu , Nano Res. 2010 , 3 , 271 ; b) C. Q. Chen , Y. Shi , Y. S. Zhang , J. Zhu , Y. J. Yan , Phys. Rev. Lett. 2006 , 96 , 075505 ; c) Y. Zhu , F. Xu , Q. Q. Qin , W. Y. Fung , W. Lu , Nano Lett. 2009 , 9 , 3934 ; d) H. S. Park , W. Cai , H. D. Espinosa , H. C. Huang , MRS Bull 2009 , 34 , 178 ; e) R. Agrawal , B. Peng , E. E. Gdoutos , H. D. Espinosa , Nano Lett. 2008 , 8 , 3668 .
[ 5 ] Y. Zhu , C. Ke , H. D. Espinosa , Exp. Mech. 2007 , 47 , 7 . [ 6 ] P. Poncharal , Z. L. Wang , D. Ugarte , W. A. de Heer , Science 1999 ,
283 , 1513 . [ 7 ] a) E. W. Wong , P. E. Sheehan , C. M. Lieber , Science 1997 , 277 ,
1971–1975 ; b) B. Wu , A. Heidelberg , J. J. Boland , Nat. Mater. 2005 , 4 , 525 .
[ 8 ] a) M. F. Yu , O. Lourie , M. J. Dyer , K. Moloni , T. F. Kelly , R. S. Ruoff , Science 2000 , 287 , 637 ; b) Y. Zhu , H. D. Espinosa , Proc. Natl. Acad. Sci. USA 2005 , 102 , 14503 .
[ 9 ] X. D. Li , H. S. Gao , C. J. Murphy , K. K. Caswell , Nano Lett. 2003 , 3 , 1495 .
[ 10 ] a) Y. Zhu , N. Moldovan , H. D. Espinosa , Appl. Phys. Lett. 2005 , 86 , 013506 ; b) A. V. Desai , M. A. Haque , Sens. Actuators, A 2007 , 134 , 169 .
[ 11 ] W. Q. Ding , L. Calabri , X. Q. Chen , K. M. Kohhaas , R. S. Ruoff , Compos. Sci. Technol. 2006 , 66 , 1112 .
[ 12 ] Z. L. Wang , J. Phys.: Condens. Matter 2004 , 16 , R829 . [ 13 ] W. Ding , D. A. Dikin , X. Chen , R. D. Piner , R. S. Ruoff , E. Zussman ,
X. Wang , X. Li , J. Appl. Phys. 2005 , 98 , 014905 . [ 14 ] M. R. He , Y. Shi , W. Zhou , J. W. Chen , Y. J. Yan , J. Zhu , Appl Phys
Lett 2009 , 95 , 091912 . [ 15 ] a) X. D. Bai , P. X. Gao , Z. L. Wang , E. G. Wang , Appl. Phys. Lett.
2003 , 82 , 4806 ; b) Y. H. Huang , X. D. Bai , Y. Zhang , J. Phys.: Condens. Matter 2006 , 18 , L179 .
[ 16 ] A. Soudi , E. H. Khan , J. T. Dickinson , Y. Gu , Nano Lett. 2009 , 9 , 1844 .
Received: February 10, 2012 Published online:
Supporting Information is available from the Wiley Online Library or from the author.
This work was supported by the National Science Foundation under Award Nos. CMMI-1030637 and CMMI-1129817. The authors thank Prof. Y. Gu for providing the ZnO NW samples and Prof. X. Jiang for providing the piezoelectric sheet.
rlag GmbH & Co. KGaA, Weinheim small 2012, DOI: 10.1002/smll.201200314